Fermentation based carbon nanotube multifunctional bionic composites
received: 18 February 2016
Luca Valentini1, Silvia Bittolo Bon1, Stefano Signetti2, Manoj Tripathi3, Erica Iacob3 & Nicola M. Pugno2,3,4
accepted: 12 May 2016 Published: 09 June 2016
The exploitation of the processes used by microorganisms to digest nutrients for their growth can be a viable method for the formation of a wide range of so called biogenic materials that have unique properties that are not produced by abiotic processes. Here we produced living hybrid materials by giving to unicellular organisms the nutrient to grow. Based on bread fermentation, a bionic composite made of carbon nanotubes (CNTs) and a single-cell fungi, the Saccharomyces cerevisiae yeast extract, was prepared by fermentation of such microorganisms at room temperature. Scanning electron microscopy analysis suggests that the CNTs were internalized by the cell after fermentation bridging the cells. Tensile tests on dried composite films have been rationalized in terms of a CNT cell bridging mechanism where the strongly enhanced strength of the composite is governed by the adhesion energy between the bridging carbon nanotubes and the matrix. The addition of CNTs also significantly improved the electrical conductivity along with a higher photoconductive activity. The proposed process could lead to the development of more complex and interactive structures programmed to self-assemble into specific patterns, such as those on strain or light sensors that could sense damage or convert light stimulus in an electrical signal. Microorganisms play an essential role in the biogenic of elements and in the formation of materials with unexplored properties1–3. Biogenic materials are formed in the nanometer scale through diverse metabolic activities and by passive surface reactions on cell walls or extracellular structures3. For example, it is known that acetobacter bacteria spins cellulose, a byproduct, as it consumes glucose, the reasons for which are unclear but it is thought the material might protect the bacteria colony from external contamination4. Extracellular polymeric secretions are multipurpose polymers that are important for applications in several fields. Extracellular polymeric secretions are involved in cellular associations, bacterial nutrition, and interaction of bacteria with their bio-physicochemical environment. Thus to create the material, the microorganism requires specific conditions. Yeast is a cellular factory which is able of taking simple molecules from its environment, such as sugars, and synthesize new elements needed for its growth at mild temperature5–8. Moreover, many of such microorganisms during their growth have the ability to adhere and to form a biofilm on different kinds of surfaces in nature8,9. It would be expected that a solution of nanomaterials and water, for example, can be mixed with nutrients for the microorganisms giving novel outstanding properties to the end material after the digestion process has taken place10–12. Fermentation of microorganism in the presence of nanomaterials could be a viable method to create a biogenic composite. It could be possible to get from large cultures enough material to create composites with unexpected properties13. Yeast cells are widely used in industrial and biological processes. The beer’s yeast, Saccharomyces cerevisiae, is the yeast responsible for sugar fermentation and has been used for centuries in wine and bread making. Moreover beer yeast extract is inexpensive, non-toxic, easy to prepare and abundantly available in nature14,15. Flocculation of yeast cells is defined as the phenomenon wherein yeast cells sediment rapidly from the medium in which they 1
Dipartimento di Ingegneria Civile e Ambientale, Università di Perugia, UdR INSTM, Strada di Pentima 4, I-05100 Terni, Italy. 2Laboratory of Bio-Inspired and Graphene Nanomechanics, Department of Civil, Environmental and Mechanical Engineering, University of Trento, via Mesiano 77, I-38123 Trento, Italy. 3Centre for Materials and Microsystems, Fondazione Bruno Kessler, via Sommarive 18, I-38123 Trento, Italy. 4School of Engineering and Materials Science, Queen Mary University of London, Mile End Road, E1 4NS London, United Kingdom. Correspondence and requests for materials should be addressed to L.V. (email: [email protected]
) or N.M.P. (email: [email protected]
) Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
www.nature.com/scientificreports/ are suspended and it occurs in the fermentation process when the sugar sources are exhausted16. Flocculation of microorganisms is simple, cheap and facile for thin film deposition because it does not require complex procedures. However, to the best of our knowledge, the spontaneous incorporation of nanomaterials in the inner structure of yeast cells during the fermentation, has not been achieved to date. Carbon nanotubes (CNTs) are nowadays materials produced at the industrial scale17, making them a tunable platform for mimicking what occurs in nature when cells grow on nanostructured surfaces. The mechanism of nutrition and growth of microorganism represents an unexplored field to design interface between microorganism and such nanomaterials. In several recent studies, CNTs were shown to be a very useful electron transfer for enzymatic as well as for cellular applications18. Considering the conducting nature of CNTs, the interactions between microorganism and carbon nanotubes could be used for generating bionic nanomaterials with unexpected electrical properties. Such living materials can be considered as bionic materials because they have the benefits of both biological world which can self-organize and that of non-living materials, which add functions such as electronic transport. Several cells (neurons, muscle) were found to respond to electrical signals but unfortunately are difficult to culture with procedures that are time consuming19,20. Saccharomyces cerevisiae is instead more robust and accessible fungi cell that allow fast and reliable experiments to investigate their electrical behavior when combined with conducting nanomaterials. Hence, we decided to explore their possible use in electrical applications and particularly to examine whether yeast after its fermentation and flocculation can interact in synergy with CNTs still benefiting from their electrical conductivity, high surface area, flexibility and capability to be wrapped by microorganisms. Here, we report the production of beer’s yeast cells/carbon nanotube composite directly by fermentation of the yeast extract in presence of CNT aqueous dispersion. We observe in the composite an increment of the mechanical properties with respect to the neat fermented yeast, in terms of tensile strength, Young’s and toughness moduli. The electrical and optical analysis demonstrated that fermentation of the beer’s yeast in presence of CNTs enhances the electrical conductivity as well as the photoconducting activity of the composite film. Such results could open the way to the realization and exploitation of such bionic structures for the realization of novel functional living materials.
Carbon nanotubes (NC 7000) were supplied by Nanocyl and their structure was confirmed by transmission electron microscopy (see Fig. S1 of Supporting Information) having an average diameter 9.5 nm and an average length 1.5 μm. Saccharomyces cerevisiae based commercial beer yeast extract with additives was used as the medium for fermentation. Water solution (50 mg/ml) of yeast was prepared in a sterilized flask at 110 rpm and 30 °C for 1 h. After that, sugar (i.e. sucrose) was added for the fermentation. The amount of sugar added is usually between 3 and 5 times the weight of the medium. Neat and fermented yeast were then drop into sterilized circular aluminum molds and the liquid medium was left to evaporate at 30 °C during the night. Films of circular shape were then obtained. Water dispersion of CNTs (1 mg/ml) were prepared by tip sonication. The dispersion of CNTs (1 mg/ml) was then added to the yeast solution and stirred at 110 rpm at 30 °C for 1 h. Then the yeast/CNTs solution was put into a sterilized circular aluminum mold, and the liquid medium was left to evaporate at 30 °C during the night. In another sterilized flask the same procedure was adopted by adding sugar to promote the fermentation of the yeast/CNTs solution (Fig. 1a). After fermentation, the liquid medium was dried in a sterilized mold and a composite film was obtained. Field emission scanning microscopy (FESEM) was used to investigate the cross section of the samples obtained by fracture in liquid nitrogen. Morphological characterization was carried out on films deposited on Si substrates by means of an Atomic Force Microscopy (AFM) apparatus (P47H Solver from NT-MDT) in intermittent contact mode at room temperature in air condition. A silicon cantilever with a tip radius of approximately 25 nm covered with native oxide was used. The tensile properties of films, i.e. tensile strength, fracture strength and elongation at break, were measured using a universal tensile testing machine (Lloyd Instr. LR30K) with a 50 N static load cell. The film samples were cut into strips (30 mm × 12 mm). The gauge length was 20 mm, and the extension rate was set at 2 mm/min. Ultraviolet–visible (UV–Vis) measurements of the deposited films were carried out with a Perkin-Elmer spectrometer Lambda 35; for all samples, a neat quartz slide was used as reference. The optical absorbance was obtained on films of the same thickness (~5 μm). The current–voltage characteristic was performed by a computer controlled Keithley 4200 Source Measure Unit. The electrical conductivity of the samples was monitored, at room temperature, by applying a sweeping DC electric voltage from −40 V to 40 V between the electrodes. Forward and reverse scans were performed on each sample. The photocurrent was measured under AM1.5D 150 mW/cm2 illumination from a Thermal Oriel solar simulator. Photoelectrical measurements were obtained for the films over several on/off light illumination cycles.
Results and Discussion
The scheme of our method is sketched in Fig. 1a: the yeast cells gain nutrient from the conversion of sucrose and grow with the division process in presence of sucrose/CNTs aqueous dispersion. Fig. 1b–d shows the appearance of the prepared samples. It can be seen that the fermented yeast presents a yellowish brown color similar to that of beer yeast. The fermentation assisted composite film exhibits a yellowish transparent color. Based on visual observation, the incorporation of CNTs without fermentation led to the formation of a black brittle film. The effect of fermentation and CNT addition on the morphology of the films was investigated by AFM and the results are reported in Fig. 2. The shape of the cells was found to be spheroidal. In general, the fermentation process of the yeast decreases the average surface roughness from 0.32 μm to 0.22 μm (Fig. 2a,b) accordingly to the Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
Figure 1. (a) Schematic representation and appearance of the fermentation-mediated assembly of carbon nanotubes and yeast cells. Photo images of (b) fermented yeast, (c) fermentation assisted yeast/CNTs film and (d) yeast/CNTs film without fermentation. From panel (c) it is clear that the underlying aluminum mold is well visible under white light. yeast morphology reported elsewhere21. Representative images of the samples (see Fig. S2) show a morphology consisting of aggregated yeast cells with cell boundaries being the surface of the film obtained by fermentation of yeast with CNTs more homogeneous (i. e. lower protrusions). Under FESEM with an acceleration voltage of the electron beam set to 5 kV, it can be seen clearly that almost all the yeast cells after fermentation kept their spherical shape structures (Fig. S3) with a morphology comparable with those obtained by AFM. It can be seen also from FESEM analysis that yeast cells before fermentation appeared concave and burst. This can be attributed to hyper-osmotic shock by exposure in the high vacuum and under the electron beam of FESEM. The strategy adopted for this study is based on the previous papers reporting that Saccharomyces cerevisiae multiplies with a process where a daughter cell is initiated as growth from the mother cell22. The round protrusion on the cell surface, visible in Fig. 3a, is a bud scar. The bud scar forms on the cell after the process of division has taken place. We exploit this growth process in order to verify if intracellular transport of carbon nanotubes takes place during this growth process as sketched in Fig. 1b. Stressing the composite sample by prolonged exposure under high vacuum condition and electron beam of FESEM, suggests that in the composite film obtained after fermentation the CNTs are bridging the yeast cells and are internalized by them (Fig. 3b,c). Such results are in agreement with those found by Zhou et al.23 who showed that CNTs did not remain on the outside membrane but transverse the membranes and localized in the cell. Moreover the formation of CNT bundles between the cell walls reported below in Fig. 3d–f for the yeast/CNTs sample without fermentation, indicates that when the CNT are not digested by the yeast cell, they behave as defects making fragile and brittle the composite film as reported below. Microscopy studies demonstrate that this approach can be regarded as the effective and versatile way to create hybrid micro-bubbles. After the FESEM inspection, we suggest that the bridging promoted by the internalized CNTs might result in additional mechanical properties to those composites according to the pull-out sketch reported in Fig. S4. In this regard tensile tests were performed and the stress-strain curves of the prepared samples are reported in Fig. 4a,b. The values of fracture strength (i. e. the stress at the ultimate strain), the elongation at break (i. e. the ultimate strain), the toughness (i.e. the area underlying the stress-strain curves) and elastic moduli are reported in Fig. S4. Generally, it was observed that the fracture strength, toughness and elastic modulus increase when CNTs were added to the yeast. The incorporation of CNTs before fermentation demonstrated to produce the highest variation in tensile properties of the composite film, being this effect highest for fracture strength; this led to extremely fragile film with the lowest elongation break value (see Figs 4b and S5). This result is consistent with our finding reported above based on visual appearance of the composite film on the mold as reported in Fig. 1. On the contrary, the composite film obtained after fermentation showed both a lower fracture strength and elastic modulus with a significantly higher elongation at break (Figs 4b and S5). The increase of elongation at break after fermentation, can be attributed to a decrease in film density and thus to an increase of the mean free volume of the film24,25. The tensile test results can be rationalized assuming a pull out model26–28 representing the failure mechanisms of bridging nanotubes at cell interface (Fig. S4). The tensile strength of the Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
Figure 2. 2D and 3D AFM topography images of (a) yeast/CNTs and (b) fermented yeast/CNTs composite films.
composite, σf, can be expressed as the combination of the strength of the matrix constituted by the yeast, σf-yeast, and the pull out strength of CNTs, σf-cntpo, according to the following rule of mixture like equation: σ f = f σ f ‐cntpo + (1 − f ) σ f ‐yeast
where f is the volume (areal) fraction of CNTs bridging the interface of the yeast cells. For f = 0 we get the strength of the matrix (i.e. σf = σf-yeast). We estimate from FESEM (Fig. 3b and detail in Supplementary Fig. 3S) observation f = 0.0205 and tensile strength values of 0.240 MPa and 0.297 10−1 MPa for σf (i.e. the fermented composite) and for σf-yeast (i.e. the fermented yeast), respectively, obtaining a σf-cntpo of 10.29 MPa. From this calculation we found that the σf-yeast 1
Figure 4a,b shows the superposition of the FEM simulations on experimental curves. In particular Fig. 4a shows the results for mother-daughter cells in fermented yeast, while in Fig. 4b the cases of equal cells with CNTs before fermentation and mother-daughter cells with CNTs after fermentation were considered. The obtained results are in good agreement with experiments, following the variation in the peak tensile stress and ultimate strain. In particular the best match between the simulated and real curves occurs for volume fraction values of fy+CNTs = 0.071 and fy+CNTs,ferm = 0.019 for yeast/CNTs and fermented yeast/CNTs composites, respectively. Note that the latter value is comparable with the one estimated from the SEM images (Fig. 3b) and assumed in the pull-out model. This result is interpreted with a higher contact area of the yeast cell-cell interface due to the increase of the cell volume after fermentation. The consequent drop of the volume fraction of the nanotubes explains the lower failure stress and the higher failure strain observed for the composite film after fermentation. This suggests further investigations for understanding the interface transformation mechanism upon fermentation. Once collected the morphology and the mechanical properties of the films, we next investigated the electrical characteristics of the composite films, and assess how they compare with the native films made of neat yeast. This
Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
Figure 5. I-V characteristics of the prepared samples.
filled and bridged microenvironment could be a viable network for enhancing the electron transfer through the nanocomposite. Thus we investigate whether there is any advantage to add CNTs to the yeast in terms of electrical conductivity. Current-voltage characteristic was thus used to measure the conductivity of yeast modified with CNTs as reported in Fig. 5. We observed that the increase in conductivity is more prominent with the CNTs. We further observed that the addition of sucrose to the neat yeast resulted in a better conductivity being this effect more pronounced for the fermented yeast/CNTs system. The source of this behavior is the bridging of CNTs of the yeast during the fermentation that improved the percolation pattern for electron transfer to the electrodes, via the conducting capabilities of CNTs. On the contrary the formation and confinement of isolated CNT bundles between the cell walls (Fig. 3d–f) results in an interruption of the percolation pattern leading to a lower conductivity for the yeast/ CNTs sample without fermentation. The peaks observed for forward and reverse voltage scans for the fermented samples, could be attributable to the reduction and oxidation activity of the sucrose oxidase in the composite films31. Further investigations into electrochemical properties of such systems are underway. Light absorbance in the UV–Vis range of the prepared samples are presented in Fig. 6a. In the visible range (350–800 nm), depending on both the CNTs incorporation and fermentation process, differences were obtained in terms of normalized optical absorbance. The absorbance value for the yeast film incorporating CNTs relative to neat yeast shows a significant increase. This difference may be associated with the presence of an extended network of aggregated CNTs that blocked passage of visible light in a more effective way. The fermentation of the yeast in presence of CNTs resulted in a decrease of the optical absorbance indicating a better dispersion and/or confinement of the CNT bundle, thus resulting in a better transparency of the composite film. In previous studies food pigments extracted from yeast fermentations have been studied as a novel sensitizing dye for dye-sensitized solar cells32–34. Moreover, Hildebrandt et al.35 recorded photocurrents and photovoltages with yeast plasma membrane attached to a planar lipid membrane and to a polytetrafluoroethylene (Teflon) film, respectively. In Fig. 6b the photocurrents that evolve before and after light exposure on the prepared samples are reported. It is clear from the curves that neat yeast as well as fermented yeast showed a current increase under illumination. The spectral irradiance for a Xenon lamp between 400 and 500 nm under the AM1.5D standard condition is about 16.9%; the absorption spectrum of the films in this optical window (i. e. 416 nm from Fig. 6a) supports the observation that a photocurrent signal for the yeast extract has been recorded. It is important to note that when the same experiment was conducted in the presence of CNTs, the baseline of the dark current signal increases, being this effect more pronounced for the composite film obtained after fermentation. The photo response, estimated as the relative variation between the dark and the light signals, increases from 16% to 26% when the fermented yeast was compared with the composite obtained after fermentation. The mechanism is related to a lower surface roughness of the composite film obtained by fermentation that promotes a more favorable charge transfer from the yeast cell to the CNTs. In particular, it is generally acknowledged that for a solution-processed active interface, in which an insulating/dielectric material (i.e. yeast in our case) is deposited from solution with a solution-processable conducting material (i.e. CNTs in our case) the interfacial mixing Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
Figure 6. (a) UV-VIS spectra of the prepared films. (b) Photocurrent recorded on the prepared samples when the films were exposed to illumination cycles. The change of the current intensity represents the switching on and off of the solar simulator (i. e. 3, 6, 6 and 3 cycles for the yeast, yeast after fermentation, yeast/CNTs and yeast/CNTs after fermentation, respectively). generally lead to increased interface roughness. The correlation between interface roughness and charge mobility in solution-processed films has been investigated by Sirringhaus et al.36,37, who developed a modeling approach for conducting–dielectric interface demonstrating that the charge mobility was found to be constant for certain values of the interface roughness less than a critical threshold. For roughness exceeding this threshold, a very rapid drop of the mobility by orders of magnitude was observed.
In this work composite films were successfully prepared by the fermentation of beer yeast in presence of carbon nanotubes. The process produced marked enhancement in mechanical properties of the composite film. This change was ascribed to a bridging mechanism promoted by the living digestion of CNTs. The composite resulting from fermentation showed an improved electrical conductivity along with an enhanced photoconducting activity. In summary we demonstrated the development of novel structures by means of biogenesis without the post-synthesis addition of the inorganic components by physical or chemical methods. In this context the present work aims the development of future applications of such bionic materials, e.g. in the manufacture of physical smart objects with multifunctional properties, in the fields of functional tissues, energy storage and light harvesting applications.
1. Newman, D. K. Microbiology - How bacteria respire minerals. Science 292, 1312–1313 (2001). 2. Lowenstam, H. A. Minerals formed by organisms. Science 211, 1126–1131 (1981). 3. Fortin, D. What biogenic minerals tell us. Science 303, 1618–1619 (2004). 4. Klemm, D., Schumann, D., Udhardt, U. & Marsch, S. Bacterial synthesized cellulose - artificial blood vessels for microsurgery. Progress in Polymer Science 26, 1561–1603 (2001). 5. Chen, Y., Daviet, L., Schalk, M., Siewers, V. & Nielsen, J. Establishing a platform cell factory through engineering of yeast acetyl-CoA metabolism. Metab. Eng. 15, 48–54 (2013). 6. Hong, K. K. & Nielsen, J. Metabolic engineering of Saccharomyces cerevisiae: a key cell factory platform for future biorefineries. Cell. Mol. Life Sci. 69, 2671–2690 (2012). 7. Runguphan, W. & Keasling, J. D. Metabolic engineering of Saccharomyces cerevisiae for production of fatty acid-derived biofuels and chemicals. Metab. Eng. 21, 103–113 (2014). 8. Everaert, E. P. J. M., van der Mei, H. C. & Busscher, H. J. Adhesion of yeasts and bacteria to fluoro-alkylsiloxane layers chemisorbed on silicone rubber. Colloids and Surfaces B: Biointerfaces 10, 179–190 (1998). 9. Neu, T. R., van der Mei, H. C., Busscher, H. J., Dijk, F. & Verkerke, G. J. Biodeterioration of medical-grade silicone-rubber used for voice prostheses - a SEM study. Biomaterials 14, 459–464 (1993). 10. Gugerli, R., Breguet, V., Stockar, U. & Marison, I. W. Immobilization as a tool to control fermentation in yeast-leavened refrigerated dough. Food Hydrocolloids 18, 703–715 (2004). 11. Jones, R. P. & Greeneld, P. F. Effect of carbon dioxide on yeast growth and fermentation. Enzyme Microb. Technol. 4, 210–223 (1982). 12. Zhang, Q. et al. Microorganism inspired hydrogels: hierarchical super/macro-porous structure, rapid swelling rate and high adsorption. RSC Adv. 4, 32475–32481 (2014). 13. Nout, M. J. R. Encyclopedia of Food Safety 3, 168 (2014). 14. Mitchell, D. N., Godwin, H. A. & Claudio, E. Nonoparticle toxicity in saccharomyces cerevisiae: a comparative study using au colloid, Ag colloid, and HAuCl4.3H2O in solution. Nanoscape 1, 59–69 (2004). 15. Kasemets, K., Ivask, A., Dubourguier, H.-C. & Kahru, A. Toxicity of nanoparticles of ZnO, CuO and TiO2 to yeast Saccharomyces cerevisiae. Toxicity in Vitro 23, 1116–1122 (2009). 16. Kourkoutas, Y., Bekatorou, A., Banat, I. M., Marchant, R. & Koutinas, A. A. Immobilization technologies and support materials suitable in alcohol beverages production: a review. Food Microbiol. 21, 377–397 (2004). 17. Zhang, X. et al. Ultrastrong, stiff, and lightweight carbon-nanotube fibers. Adv. Mater. 19, 4198 (2007). 18. Karajanagi, S. S., Vertegel, A. A., Kane, R. S. & Dordick, J. S. Structure and function of enzymes adsorbed onto single-walled carbon nanotubes. Langmuir 20, 11594–11599 (2004). 19. Requena, J., Whittembury, J., Scarpa, A., Brinley Jr., J. F. & Mullins, L. J. Intracellular ionized calcium changes in squid giant-axons monitored by fura-2 and aequorin. Ann. N. Y. Acad. Sci. 639, 112–125 (1991).
Scientific Reports | 6:27031 | DOI: 10.1038/srep27031
www.nature.com/scientificreports/ 20. Watanabe, A. & Endoh, M. Relationship between the increase in Ca2 + transient and contractile force induced by angiotensin II in aequorin-loaded rabbit ventricular myocardium. Cardiovasc. Res. 37, 524–531 (1998). 21. Ahmad, M. R., Nakajima, M., Kojima, S., Homma, M. & Fukuda, T. In situ single cell mechanics characterization of yeast cells using nanoneedles inside environmental SEM. IEEE Transactions on Nanotechnology 7, 607–616 (2008). 22. Broach, J. R., Jones, E. W. & Pringle, J. R. The Molecular and Cellular Biology of the Yeast Saccharomyces, Vol. 1. Genome Dynamics, Protein Synthesis, and Energetics. Cold Spring Harbor, NY: Cold Spring Harbor Laboratory Press; (1991). 23. Zhou, F. et al. Periodic ZnO nanorod arrays defined by polystyrene microsphere self-assembled monolayers. Nano Letters 6, 2375–2378 (2006). 24. Gontard, N., Duchez, C., Cuq, J. L. & Guilbert, S. Edible composites films of wheat gluten and lipids: water vapor permeability and other physical properties. Int. Journal of Food Science Technol. 29, 39–50 (1994). 25. Yang, L. & Paulson, A. T. Effects of lipids on mechanical and moisture barrier properties of edible gellan film. Food Research International 33, 571–578 (2000). 26. Pugno, N. The design of self-collapsed super-strong nanotube bundles. J. of the Mechanics and Physics of Solids 58, 1397–1410 (2010). 27. Pugno, N. Mimicking nacre with super-nanotubes for producing optimized super-composites. Nanotechnology 17, 5480–5484 (2006). 28. Shi, X., Peng, B., Pugno, N. M. & Gao, H. Stretch-induced softening of bending rigidity in graphene. Applied Physics Letters 100, 191913–191915 (2012). 29. Belytschko, T., Liu, W.-K., Moran, B., Elkhodary, K. Nonlinear Finite Element for Continua and Structures, 2nd Ed.. John Wiley & Sons, Ltd.; (2014). 30. Hartmann, C. & Delgado. A. Numerical simulation of the mechanics of a yeast cell under high idrostatic pressure. Journal of Biomechanics 37, 977–978 (2004). 31. Wu, X. et al. Direct electron transfer of glucose oxidase immobilized in an ionic liquid reconstituted cellulose-carbon nanotube matrix. Bioelectrochemistry 77, 64–68 (2009). 32. Zhang, G. et al. High efficiency and stable dye-sensitized solar cells with an organic chromophore featuring a binary pi-conjugated spacer. Chem. Commun. 16, 2198–2200 (2009). 33. Hwang, S. et al. A highly efficient organic sensitizer for dye-sensitized solar cells. Chem. Commun. 14, 4887–4889 (2007). 34. Ito, S. et al. High-efficiency organic-dye-sensitized solar cells controlled by nanocrystalline-TiO2 electrode thickness. Adv. Mater. 18, 1202 (2006). 35. Hildebrandt, V. et al. Bacteriorhodopsin expressed in schizosaccharomyces-pombe pumps protons through the plasma-membrane. Proc. Natl. Acad. Sci. USA 90, 3578–3582 (1993). 36. Chua, L. L., Ho, P. K. H., Sirringhaus, H. & Friend R. H. Observation of field-effect transistor behavior at self- organized interfaces. Adv. Mater. 16, 1609–1613 (2004). 37. Sirringhaus H. Device physics of solution-processed organic field-effect transistors. Adv. Mater. 17, 2411–2425 (2005).
NMP is supported by the European Research Council (ERC StG Ideas 2011 BIHSNAM n. 279985, ERC PoC 2015 SILKENE nr. 693670) and by the European Commission under the Graphene Flagship (WP14 “Polymer nanocomposites”, n. 696656). SS acknowledges support from BIHSNAM.
L.V. and N.M.P. had the idea, designed and supervised the entire research and analyzed the results. S.B.B. prepared the samples and performed the morphological, electrical and UV-Vis characterizations. M.T. and E.I. performed AFM analysis and scratch tests. S.S. performed FEM simulations. S.S. and N.M.P. rationalized the mechanical results. All authors have revised and given their approval to the final version of the manuscript.
Supplementary information accompanies this paper at http://www.nature.com/srep Competing financial interests: The authors declare no competing financial interests. How to cite this article: Valentini, L. et al. Fermentation based carbon nanotube multifunctional bionic composites. Sci. Rep. 6, 27031; doi: 10.1038/srep27031 (2016). This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
Scientific Reports | 6:27031 | DOI: 10.1038/srep27031